Post on 14-Apr-2016
Embed Size (px)
ISSN: 0973-4945; CODEN ECJHAO E-Journal of Chemistry
http://www.e-journals.net Vol. 5, No. 1, pp. 81-85, January 2008
Production of Cellulosic Polymers from Agricultural Wastes
A.U. ISRAEL, I.B. OBOT*, S. A. UMOREN, V. MKPENIE and J.E. ASUQUO
Department of Chemistry,Faculty of Science, University of Uyo, P.M.B. 1017, Uyo, Nigeria.
Received 12 May 2007; Accepted 10 July 2007
Abstract: Cellulosic polymers namely cellulose, di-and triacetate were produced from fourteen agricultural wastes; Branch and fiber after oil extraction from oil palm (Elais guineensis), raffia, piassava, bamboo pulp, bamboo bark from raphia palm (Raphia hookeri), stem and cob of maize plant (Zea mays), fruit fiber from coconut fruit (Cocos nucifera), sawdusts from cotton tree (Cossypium hirsutum), pear wood (Manilkara obovata), stem of Southern gamba green (Andropogon tectorus), sugarcane baggase (Saccharium officinarum) and plantain stem (Musa paradisiaca). They were subjected to soda pulping and hypochlorite bleaching system. Results obtained show that pulp yield from these materials were: 70.00, 39.59, 55.40, 86.00, 84.60, 80.00, 40.84, 81.67, 35.70, 69.11, 4.54, 47.19, 31.70 and 52.44% respectively. The pulps were acetylated with acetic anhydride in ethanoic acid catalyzed by conc. H2SO4 to obtain cellulose derivatives (Cellulose diacetate and triacetate). The cellulose diacetate yields were 41.20, 17.85, 23.13, 20.80, 20.23, 20.00, 39.00, 44.00, 18.80, 20.75, 20.03, 41.20, 44.00, and 39.00% respectively while the results obtained as average of four determinations for cellulose triacetate yields were: 52.00, 51.00, 43.10, 46.60, 49.00, 35.00, 40.60, 54.00, 57.50, 62.52, 35.70. 52.00, 53.00 and 38.70% respectively for all the agricultural wastes utilized. The presence of these cellulose derivatives was confirmed by a solubility test in acetone and chloroform.
Keywords: Cellulose polymers, Proximate composition, Pulping, Acetylation.
Introduction Many agricultural by-products from agricultural activities and agro-based processing litter the environments and constitute waste problems. This research is aimed at converting some of these unwanted agricultural waste or by-products to commercially useful products such as pulp and cellulose acetate. This work has the potential of providing new market and applications for low value and utilized agricultural wastes by converting into cellulose acetate. The principle
82 I.B. OBOT et al.
behind the research is that most agricultural by-products are composed of cellulose in the plant cell walls. Cellulose (C6H10O5)n is a large chain polymeric polysaccharide carbohydrate of beta-glucose. The principal functional groups in pure cellulose are hydroxy (-OH) making cellulose a polyol with primary and secondary alcohol functional groups (-CH2OH, -CHOH). The multiple hydroxy groups of cellulose in cellulosic materials (agro-waste) can be partially or wholly modified by reacting with various chemicals to produce a wide range of end products referred to as cellulose derivatives. These derivatives such as cellulose nitrates, acetates, xanthates, ethers, rayon and cellophanes have far reaching industrial applications. Cellulose nitrate has the largest industrial use as lacquer coating for decorative and protective purposes. It is also useful in the photographic industry, in explosives and propellants1-4. Among all cellulose derivatives, cellulose acetate as by far been recognized as the most important organic ester of cellulose owing to its extensive industrial and commercial importance. It has many uses such as in the production of plastics films, lacquers, photographic films, thermoplastic moulding, transparent sheeting, camera accessories, magnetic tapes, combs, telephone, and electrical parts 5-7. The production of cellulose acetate from agro-waste such as jute stick, cotton linters, woodchips, rice straw, wheat hull and corn fiber have been reported in literature8,1,7. In Nigeria, enormous volumes of agricultural wastes that contain cellulosic fibers are generated annually. Many of these agro-wastes are allowed to rot away utilized. For example, tonnes of maize stem, cobs from Zea mays, plantain stem, raffia from Raphia hookeri are allowed to rot away yearly and eventually polluting the environment. These agricultural wastes can be gainfully utilized in the production of pulp for papermaking and conversion to cellulose derivatives for manufacture of plastics, photographic films etc. This will not only encourage local farmers as new market is developed for materials but will also boost the Nigerian economy. Also the problem of environmental pollution arising from the decay of these materials will be minimized. Recently, our research group has reported on the conversion of some agricultural wastes to cellulose derivatives7. The present work is another trial aimed at practically exploiting these biodegradable agricultural wastes materials as a potential alternative for the production of pulps and subsequent conversion to cellulose derivatives.
Experimental Agricultural wastes used were branch, fiber after oil extraction of Elais guineensis (oil palm tree), fiber of Cocos nucifera, raffia, bamboo pulp and bark from Raphia hookeri, maize cob and stem from Zea mays, sawdust from Manilkara obovate (pear wood), sawdust from Gosspium hirsutum (cotton tree), stem from Andropogon tectoris (Southern gamba grass) and stem of Musa paradisiaca (plantain). They were obtained from Uyo area of Akwa Ibom State, Nigeria and authenticated by a botanist in the Department of Botany, University of Uyo, Nigeria. Chemical/ reagents used were Analar grade and were therefore used without further purification. The samples were allowed to dry and thereafter were sliced into small pieces and beaten to reduce the filaments for further analysis.
Proximate compositions, moisture content, solubility in 1% NaOH, cellulose content were determined using standard methods of the Association of Official Analytical Chemist10. The presence of lignin and rosin in the samples were detected using phloroglucinol solution and Hierberman-starch method respectively3.
The pulping process employed was the soda pulping method. 10.0g of each of the sample were boiled with 200.0 mL of 18% NaOH solution for one hour. The resulting mixture was
Production of Cellulosic Polymers from Agricultural Wastes 83
filtered off and washed with distilled water to free the fibers (defibiring). The samples were collectively bleached using hypochlorite in alkaline medium. The bleached samples were dried at 805 oC in the oven for 8 h to give cellulose pulp. Moisture content of the wet pulp and pulp yield were estimated.
Preparation of Cellulose Acetates 2.0g of each of the dried bleached pulp was dispersed in 35mL of glacial acetic acid. The solution was kept in water bath between 50-55 oC for one hour with frequent stirring. An acetylating mixture of 0.4mL conc. H2SO4 and 10mL of acetic anhydride was gradually added to the glacial acetic acid-pulp mixture, keeping the temperature between 605 oC. The resulting mixture was kept in water bath for an hour at 50-55 oC with occasional stirring until a clear solution was obtained. The clear solution was divided into two portions: to one-half were precipitated triacetate and other portion diacetate. The precipitates was filtered and washed thoroughly until it was neutral to litmus. The precipitates were dried and subjected to solubility test in chloroform and acetone to confirm their presence. The solubility properties of cellulose diacetate and triacetate in chloroform and acetone as well as their yields were determined.
Results and Discussion The results of the proximate composition, cellulose content, pulp yields, moisture contents of the pulp and cellulose derivatives yield of the agricultural wastes under investigation are presented in Table 1 & 2. From the table, the moisture content of the air-dried samples in % were 47.50, 28.90,14.20, 42.00, 36.00, 10.70 46.00, 45.00, 30.20, 41.00, 57.70, 39.78, 16.88 and 50.00% respectively for branch and fiber after oil extraction from oil palm (Elais guineensis), raffia, piassava, bamboo pulp, bamboo bark from raphia palm (Raphia hookeri), stem and cob of maize plant (Zea mays), fruit fiber from coconut fruit (Cocos nucifera), sawdusts from cotton tree (Cossypium hirsutum), pear wood (Manilkara obovata), stem of Southern gamba green (Andropogon tectorus), sugarcane baggase (Saccharium officinarum) and plantain stem (Musa paradisiaca). The lower the moisture content of the agricultural waste, the higher the fiber content of the sample. The low moisture content of raffia and bamboo bark from Raphia hookeri show the high fiber contents of these samples7.
Table 1. Proximate Composition and Acetate Yield of Some Agricultural Waste Materials. Elais
guineensis Raffia hookeri Zea mays Assay Branch Fruit fiber Raphia Piassava
Bambo bark Stem Cob
Moisture content, % 47.50 28.90 14.20 42.00 36.00 10.70 46.00 45.00 Solubility in hot
water, % 15.50 10.00 6.85 10.75 10.00 12.50 17.50 15.00 Solubility in 1%
NaOH, % 30.00 13.90 48.90 25.20 28.90 60.00 30.00 35.00 Cellulose content, % 61.10 n.d 39.00 63.00 58.00 49.50 60.00 60.00
Pulp yield, % 70.00 39.59 55.40 86.00 84.60 80.00 40.84 81.67 Moisture content of
wet pulp, % 70.00 68.70 71.50 80.00 76.50 75.50 53.50 53.50 Cellulose diacetate, % 41.20 17.85 23.13 20.80 20.23 20.00 39.00 44.00
Cellulose Triacetate, % 52.00 51.00 43.10 46.60 49.00 35.00 40.60 40.60
84 I.B. OBOT et al.
Table 2. Proximate Composition and Acetate Yield of Some Agricultural Waste Materials.